received: 20 May 2016 accepted: 10 August 2016 Published: 07 September 2016
Nucleation and strain-stabilization during organic semiconductor thin film deposition Yang Li1, Jing Wan1, Detlef-M. Smilgies2, Nicole Bouffard3, Richard Sun4 & Randall L. Headrick1 The nucleation mechanisms during solution deposition of organic semiconductor thin films determine the grain morphology and may influence the crystalline packing in some cases. Here, in-situ optical spectromicroscopy in reflection mode is used to study the growth mechanisms and thermal stability of 6,13-bis(trisopropylsilylethynyl)-pentacene thin films. The results show that the films form in a supersaturated state before transforming to a solid film. Molecular aggregates corresponding to subcritical nuclei in the crystallization process are inferred from optical spectroscopy measurements of the supersaturated region. Strain-free solid films exhibit a temperature-dependent blue shift of optical absorption peaks due to a continuous thermally driven change of the crystalline packing. As crystalline films are cooled to ambient temperature they become strained although cracking of thicker films is observed, which allows the strain to partially relax. Below a critical thickness, cracking is not observed and grazing incidence X-ray diffraction measurements confirm that the thinnest films are constrained to the lattice constants corresponding to the temperature at which they were deposited. Optical spectroscopy results show that the transition temperature between Form I (room temperature phase) and Form II (high temperature phase) depends on the film thickness, and that Form I can also be strainstabilized up to 135 °C. Methods for solution deposition of organic semiconductor thin films have proven to be far superior to vapor deposition methods in many respects, such as the ability to create oriented films with extremely large crystalline grain size and exceptional carrier mobility1–5. However, the specific crystallization processes remain largely unknown, and no clear consensus has emerged on the mechanisms behind the stabilization of metastable polymorphs3,6,7. Classical nucleation theory posits that critical nuclei grow via attachment of monomers from supersaturated solution, while subcritical nuclei tend to thermally dissociate8. However, there is abundant evidence that a two-step process, where crystals grow via attachment of pre-nucleation clusters, takes place in a diverse range of materials systems9–11. In addition, delayed crystallization from a supersaturated solution12–15, and evidence for aggregation that is not correlated to crystal diffraction16–18 have been observed in the context of drying of polymer thin films and polymer blends. Deposition on heated substrates poses an additional challenge since the stable state at the deposition temperature can become metastable once the temperature is changed, typically to ambient conditions. Here, we seek to understand both of these critical steps in the solution deposition process–nucleation and metastable state stabilization–by performing a combination of in-situ and post-deposition characterization experiments. It is widely appreciated that molecular packing strongly affects the electronic couplings between neighboring molecules in solid materials, resulting in substantial peak shifts in absorption spectra relative to isolated molecules19,20. However, there have been relatively few reports of in-situ optical spectroscopy to monitor dynamic processes during solidification of organic semiconductor thin films12,17,21–23. Since the performance of electronic devices is heavily dependent on thin film morphology and structure, understanding and control of molecular self-assembly has significant practical implications. Moreover, understanding the effect of strain on the properties of small-molecule based organic semiconductors has recently emerged as an area of fundamental and practical importance24,25. 1
Department of Physics and Materials Science Program, University of Vermont, Burlington VT 005, USA. 2Cornell High Energy Synchrotron Source, Cornell University, Ithaca NY 14853, USA. 3Microscopy Imaging Center, College of Medicine, University of Vermont, Burlington VT 05405, USA. 4Angstrom Sun Technologies Inc. 31 Nagog Park, Acton MA 01720, USA. Correspondence and requests for materials should be addressed to R.L.H. (email: [email protected]
) Scientific Reports | 6:32620 | DOI: 10.1038/srep32620
www.nature.com/scientificreports/ In this paper, we demonstrate the application of real-time optical spectroscopy to study the crystallization process and polymorphic transformation of 6,13-bis(triisopropylsilylethynyl) pentacene (TIPS-pentacene) thin films. TIPS-pentacene is one of the most heavily studied prototypical organic semiconductors because of its solution processability and excellent device performance. It has previously been reported that that the π − π ⁎ absorption features of static TIPS-pentacene thin films are broadened and red shifted compared to solution spectra by as much as 40 nm26,27. We utilize in-situ optical spectroscopy to show that TIPS-pentacene crystallizes in a two-step process, where in the first step the film exists in a supersaturated form with no long range order, as reported previously based on in-situ synchrotron X-ray scattering and Polarized Optical Video Microscopy (POVM) results3. We report evidence that TIPS-pentacene molecules aggregate into small clusters in the supersaturated form. Thus, molecular ordering begins in the first stage of the film self-assembly process as a precursor to the development of long-range ordering. Cour et al.3 have shown that strained small molecule organic semiconductor thin films can be obtained by solution deposition at elevated temperatures (60 °C and 90 °C for TIPS-pentacene). The strain is introduced after the deposition when the sample temperature is changed, as a result of the very large thermal expansion coefficient of the solid film relative to typical substrate materials such as silicon and glass3. Highly strained films are obtained after cooling unless the strain is relieved by cracking or buckling. In addition, TIPS-pentacene undergoes a bulk phase transition at 124 °C28. It has also been reported that it is possible to stabilize thin films in the high temperature phase, known as Form II, to ambient conditions4. Here, we report that in-situ optical spectroscopy is highly sensitive to changes in molecular packing and to thermal expansion effects. We utilize this effect during thermal cycling in combination with X-ray diffraction measurements to verify that Form II TIPS-pentacene films deposited at 135 °C can be stabilized to room temperature if the film thickness is below the critical thickness for cracking. We have also performed similar experiments on room temperature phase (Form I) TIPS-pentacene thin films written at 25 °C. No phase transition occurs even when the sample is heated to 135 °C, which provides confirmation of the strain-stabilization model since no reduction of the transition temperature is observed.
Results and Discussion
In situ optical monitoring of the crystallization process. Wo et al.29,30 have shown that the film morphology prepared by the hollow pen writing method is highly dependent on the writing speed. A schematic of the process is shown in Fig. 1(a). At low writing speed (25 °C) depositions. Either silicon wafers [Figs 1(c) and 2(d,e)] or glass slides [Figs 4,5 and 7(a)] were used as substrates for thin films fabricated for spectroscopy measurements and for unpolarized microscopy. Silicon with a 300 nm thermally grown silicon oxide layer was also used as substrates for polarized microscopy experiments since the grain structure contrast is enhanced due to an optical interference effect produced by the oxide layer. The substrates were sonicated in toluene, acetone, and isopropanol for 7 min. and then treated with phenyltrichlorosilane (PTS, ≥97%, Sigma Aldrich) to ensure proper wetting for the TIPS-pentacene solution. PTS treatment was accomplished by immersing the cleaned wafer or glass slide into a toluene solution of 3 wt% PTS and heated to 110 °C for 15 h under a Nitrogen overpressure to prevent evaporation of the solvent. After PTS treatment, the substrates were sonicated in toluene, acetone and isopropanol for 1 min. each. A polarizing optical microscope (Olympus BXFM) with ultra-long working distance objective lenses is used to observe the thin film growth in real-time. The system includes an integrated UV-Vis spectrometer (Angstrom Sun Technologies Inc.) to acquire reflectance spectra over a selected small area, as shown in Fig. 1. Spectra were converted to absolute reflection percentage by comparion with a silicon mirror with a well-known reflectivity. A silicon mirror was placed behind the glass substrates [Figs 4,5 and 7(a)], which serves to improve the signal and absorption contrast, as well as reducing peak shifts due to index of refraction dispersion. In the hollow capillary writing process, deposition is carried out by allowing the solution held in a rectangular capillary to make contact with the substrate, followed by lateral translation of the substrate at a constant writing speed1. The sample is mounted on a thermoelectric module for temperature control. Heating at cooling rates are about 30 °C/min unless otherwise noted. In-situ micro beam grazing incidence wide angle X-ray diffraction (μGIWAXS) was performed at the Cornell High Energy Synchrotron Source (CHESS) on the D1 beamline. X-rays with an energy of 10.74 keV (λ = 1.15 Å) were focused to a beam size of 20 μm × 20 μm using a single-bounce X-ray capillary38. The incidence angle was 0.14° and the scattering patterns were recorded using a Pilatus 200K area detector with a pixel size of 172 μm. Si/SiO2 wafers were used as substrates for all of the X-ray experiments Fig. 7(b,c) and Table 3. Film morphology and film thickness were characterized by atomic force microscopy (AFM).
1. Headrick, R. L., Wo, S., Sansoz, F. & Anthony, J. E. Anisotropic mobility in large grain size solution processed organic semiconductor thin films. Applied Physics Letters 92, 063302, doi: 10.1063/1.2839394 (2008). 2. Minemawari, H. et al. Inkjet printing of single-crystal films. Nature 475, 364–367, doi: 10.1038/nature10313 (2011). 3. Cour, I. et al. Origin of stress and enhanced carrier transport in solution-cast organic semiconductor films. Journal of Applied Physics 114, 093501, doi: 10.1063/1.4820384 (2013). 4. Diao, Y. et al. Solution coating of large-area organic semiconductor thin films with aligned single-crystalline domains. Nature Materials 12, 665–671, doi: 10.1038/nmat3650 (2013). 5. Niazi, M. et al. Solution-printed organic semiconductor blends exhibiting transport properties on par with single crystals. Nature communications 6, 8598, doi: 10.1038/ncomms9598 (2015). 6. Diao, Y. et al. Understanding polymorphism in organic semiconductor thin films through nanoconfinement. Journal of the American Chemical Society 136, 17046–17057, doi: 10.1021/ja507179d (2014). 7. Giri, G. et al. One-dimensional self-confinement promotes polymorph selection in large-area organic semiconductor thin films. Nature communications 5, 3573, doi: 10.1038/ncomms4573 (2014). 8. Porter, D. A., Easterling, K. E. & Sherif, M. Y. Phase Transformations in Metals and Alloys. 3rd edn (CRC Press, 2009).
Scientific Reports | 6:32620 | DOI: 10.1038/srep32620
www.nature.com/scientificreports/ 9. Erdemir, D., Lee, A. Y. & Myerson, A. S. Nucleation of crystals from solution: Classical and two-step models. Accounts of Chemical Research 42, 621–629, doi: 10.1021/ar800217x (2009). 10. Gebauer, D., Kellermeier, M., Gale, J. D., Bergström, L. & Cölfen, H. Pre-nucleation clusters as solute precursors in crystallisation. Chemical Society Reviews 43, 2348–2371, doi: 10.1039/C3CS60451A (2014). 11. Ito, F. et al. Direct visualization of the two-step nucleation model by fluorescence color changes during evaporative crystallization from solution. Scientific Reports 6, 22918, doi: 10.1038/srep22918 (2016). 12. Wang, T. et al. The development of nanoscale morphology in polymer: fullerene photovoltaic blends during solvent casting. Soft Matter 6, 4128–4134, http://dx.doi.org/10.1039/c0sm00343c (2010). 13. Shin, N., Richter, L. J., Herzing, A. A., Kline, R. J. & DeLongchamp, D. M. Effect of processing additives on the solidification of bladecoated polymer/fullerene blend films via in-situ structure measurements. Advanced Energy Materials 3, 938–948, http://dx.doi. org/10.1002/aenm.201201027 (2013). 14. Engmann, S. et al. Real-time x-ray scattering studies of film evolution in high performing small-molecule–fullerene organic solar cells. Journal of Materials Chemistry A 3, 8764–8771, http://dx.doi.org/10.1039/c5ta00935a (2015). 15. Chou, K. W. et al. Late stage crystallization and healing during spin-coating enhance carrier transport in small-molecule organic semiconductors. Journal of Materials Chemistry C 2, 5681–5689, http://dx.doi.org/10.1039/c4tc00981a (2014). 16. Duong, D. T., Toney, M. F. & Salleo, A. Role of confinement and aggregation in charge transport in semicrystalline polythiophene thin films. Physical Review B 86, 205205, http://dx.doi.org/10.1103/PhysRevB.86.205205 (2012). 17. Richter, L. J. et al. In situ morphology studies of the mechanism for solution additive effects on the formation of bulk heterojunction films. Advanced Energy Materials 5, 1400975, doi: 10.1002/aenm.201400975 (2015). 18. Sanyal, M. et al. In situ x-ray study of drying-temperature influence on the structural evolution of bulk-heterojunction polymer–fullerene solar cells processed by doctor-blading. Advanced Energy Materials 1, 363–367, http://dx.doi.org/10.1002/ aenm.201100007 (2011). 19. Kasha, M., Rawls, H. R. & El-Bayoumi, A. M. The exciton model in molecular spectroscopy. Pure and Applied Chemistry 11, 371–392, doi: 10.1351/pac196511030371 (1965). 20. Spano, F. C. The spectral signatures of frenkel polarons in h- and j-aggregates. Accounts of Chemical Research 43, 429–439, doi: 10.1021/ar900233v (2010). 21. Peet, J., Cho, N. S., Lee, S. K. & Bazan, G. C. Transition from solution to the solid state in polymer solar cells cast from mixed solvents. Macromolecules 41, 8655–8659, http://dx.doi.org/10.1021/ma801945h (2008). 22. Duong, D. T. et al. Mechanism of crystallization and implications for charge transport in poly (3-ethylhexylthiophene) thin films. Advanced Functional Materials 24, 4515–4521, http://dx.doi.org/10.1002/adfm.201304247 (2014). 23. Abdelsamie, M., Zhao, K., Niazi, M. R., Chou, K. W. & Amassian, A. In situ uv-visible absorption during spin-coating of organic semiconductors: a new probe for organic electronics and photovoltaics. J. Mater. Chem. C 2, 3373–3381, doi: 10.1039/C3TC32077D (2014). 24. Wu, Y. et al. Strain effects on the work function of an organic semiconductor. Nature communications 7, 10270, doi: 10.1038/ ncomms10270 (2016). 25. Kubo, T. et al. Suppressing molecular vibrations in organic semiconductors by inducing strain. Nature communications 7, 11156, doi: 10.1038/ncomms11156 (2016). 26. James, D. T., Frost, J. M., Wade, J., Nelson, J. & Kim, J.-S. Controlling microstructure of pentacene derivatives by solution processing: Impact of structural anisotropy on optoelectronic properties. ACS Nano 7, 7983–7991, doi: 10.1021/nn403073d (2013). 27. Ostroverkhova, O. et al. Optical and transient photoconductive properties of pentacene and functionalized pentacene thin films: Dependence on film morphology. Journal of Applied Physics 98, 033701, doi: 10.1063/1.1949711 (2005). 28. Chen, J., Anthony, J. & Martin, D. C. Thermally induced solid-state phase transition of bis(triisopropylsilylethynyl) pentacene crystals. The Journal of Physical Chemistry B 110, 16397–16403, doi: 10.1021/jp0627877 (2006). 29. Wo, S. Study of grain structure and interfacial structure in organic semiconductor thin films. Ph.D. thesis, University of Vermont (2011). 30. Wo, S., Headrick, R. L. & Anthony, J. E. Fabrication and characterization of controllable grain boundary arrays in solution-processed small molecule organic semiconductor films. Journal of Applied Physics 111, 073716, doi: 10.1063/1.3698203 (2012). 31. Diao, Y., Shaw, L., Bao, Z. & Mannsfeld, S. C. Morphology control strategies for solution-processed organic semiconductor thin films. Energy & Environmental Science 7, 2145–2159, doi: 10.1039/C4EE00688G (2014). 32. Yamagata, H. et al. H,j-aggregate behavior of crystalline 7,8,15,16-tetraazaterrylene: Introducing a new design paradigm for organic materials. The Journal of Physical Chemistry C 118, 28842–28854, doi: 10.1021/jp509011u (2014). 33. Anthony, J. E., Brooks, J. S., Eaton, D. L. & Parkin, S. R. Functionalized pentacene: Improved electronic properties from control of solid-state order. Journal of the American Chemical Society 123, 9482–9483, doi: 10.1021/ja0162459 (2001). 34. Vekilov, P. G. The two-step mechanism of nucleation of crystals in solution. Nanoscale 2, 2346–2357, http://dx.doi.org/10.1039/ c0nr00628 (2010). 35. Chen, J. et al. Thermal and mechanical cracking in bis(triisopropylsilylethnyl) pentacene thin films. Journal of Polymer Science Part B: Polymer Physics 44, 3631–3641, doi: 10.1002/polb.21007 (2006). 36. Wan, J. et al. Transient phases during fast crystallization of organic thin films from solution. APL Materials 4, 016103, doi: 10.1063/1.4939464 (2016). 37. Kaganer, V. et al. Strain-mediated phase coexistence in heteroepitaxial films. Physical review letters 85, 341, http://dx.doi. org/10.1103/PhysRevLett.85.341 (2000). 38. Smilgies, D.-M. et al. Look fast: Crystallization of conjugated molecules during solution shearing probed in-situ and in real time by x-ray scattering. physica status solidi (RRL)-Rapid Research Letters 7, 177–179, doi: 10.1002/pssr.201206507 (2013).
The authors thank Arthur Woll for assistance with the X-ray diffraction experimental setup. This work was supported by the National Science Foundation, Division of Materials Research, Electronic and Photonic Materials Program through award DMR-1307017. The X-ray scattering research was conducted at the Cornell High Energy Synchrotron Source (CHESS) which is supported by the NSF and the National Institutes of Health/National Institute of General Medical Sciences under NSF award DMR-1332208.
Y.L. and R.H. conceived the experiments and wrote the manuscript, Y.L., J.W. and R.H. conducted the experiments, and D.S., N.B. and R.S. provided support and advice for specific measurements (X-ray diffraction, Atomic Force Microscopy, and Optical Spectroscopy, respectively). All authors reviewed the manuscript.
Supplementary information accompanies this paper at http://www.nature.com/srep Competing financial interests: The authors declare no competing financial interests. Scientific Reports | 6:32620 | DOI: 10.1038/srep32620
www.nature.com/scientificreports/ How to cite this article: Li, Y. et al. Nucleation and strain-stabilization during organic semiconductor thin film deposition. Sci. Rep. 6, 32620; doi: 10.1038/srep32620 (2016). This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/ © The Author(s) 2016
Scientific Reports | 6:32620 | DOI: 10.1038/srep32620